Output from "TOTOPOL", (version 1.92, 17 Jul 2017, Mike Treacy).

Report for the framework in file "public/tmp/tmp_194_6_98187075_FVvdfy.cif"

There are 144 T-atoms per unit cell
There are 288 O-atoms per unit cell

Framework density = 21.24 T-atoms per nm^3
Material density = 2.119 grams per cm^3 (excluding extra-framework material)
-------------------------------------------------------------------
-------------------------- T-O Analysis ---------------------------
-------------------------------------------------------------------
[Si] Ideal SiO distance = 1.610 Angstrom
T1  -- O1  = 1.6095 Angstrom
T1  -- O2  = 1.6316 Angstrom
T1  -- O3  = 1.6090 Angstrom
T1  -- O4  = 1.6280 Angstrom
      mean = 1.6195 Angstrom
        t1 = 0.021313  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.013392  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T2  -- O3  = 1.5158 Angstrom
T2  -- O5  = 1.6187 Angstrom
T2  -- O6  = 1.6262 Angstrom
T2  -- O7  = 1.6198 Angstrom
      mean = 1.5951 Angstrom
        t1 = 0.103083  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.123342  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T3  -- O4  = 1.6283 Angstrom
T3  -- O8  = 1.6157 Angstrom
T3  -- O9  = 1.5996 Angstrom
T3  -- O10 = 1.6293 Angstrom
      mean = 1.6182 Angstrom
        t1 = 0.020087  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.013177  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T4  -- O6  = 1.7201 Angstrom
T4  -- O11 = 1.6704 Angstrom
T4  -- O12 = 1.6963 Angstrom
T4  -- O13 = 1.6380 Angstrom
      mean = 1.6812 Angstrom
        t1 = 0.056063  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.041310  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T5  -- O7  = 1.6495 Angstrom
T5  -- O14 = 1.6621 Angstrom
T5  -- O15 = 1.6382 Angstrom
T5  -- O16 = 1.6408 Angstrom
      mean = 1.6477 Angstrom
        t1 = 0.029664  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.016741  (0.0 is a perfect tetrahedron)

[Si] Ideal SiO distance = 1.610 Angstrom
T6  -- O10 = 1.6377 Angstrom
T6  -- O13 = 1.6627 Angstrom
T6  -- O16 = 1.6499 Angstrom
T6  -- O17 = 1.6197 Angstrom
      mean = 1.6425 Angstrom
        t1 = 0.023480  (0.0 is a perfect SiO4 tetrahedron)
        t2 = 0.008116  (0.0 is a perfect tetrahedron)

        T-O SUMMARY
          Range  = 1.5158 A <--> 1.7201 A
          Mean   = 1.6340 A
          StdDev = 0.0367 A

       t1 Range  = 0.0201 <-- 0.0423 --> 0.1031
       t2 Range  = 0.0081 <-- 0.0360 --> 0.1233

-------------------------------------------------------------------
------------------------- O-T-O Analysis --------------------------
-------------------------------------------------------------------
O1  -- T1  -- O2  = 109.730 deg; O1  -- O2  = 3 A
O1  -- T1  -- O3  = 109.571 deg; O1  -- O3  = 3 A
O1  -- T1  -- O4  = 104.254 deg; O1  -- O4  = 3 A
O2  -- T1  -- O3  = 114.999 deg; O2  -- O3  = 3 A
O2  -- T1  -- O4  = 110.137 deg; O2  -- O4  = 3 A
O3  -- T1  -- O4  = 107.587 deg; O3  -- O4  = 3 A
       104.254 deg <-- 109.380 deg --> 114.999 deg

O3  -- T2  -- O5  =  95.881 deg; O3  -- O5  = 2 A
O3  -- T2  -- O6  =  86.602 deg; O3  -- O6  = 2 A
O3  -- T2  -- O7  = 125.149 deg; O3  -- O7  = 3 A
O5  -- T2  -- O6  = 130.444 deg; O5  -- O6  = 3 A
O5  -- T2  -- O7  = 107.560 deg; O5  -- O7  = 3 A
O6  -- T2  -- O7  = 110.952 deg; O6  -- O7  = 3 A
       86.602 deg <-- 109.431 deg --> 130.444 deg

O4  -- T3  -- O8  = 109.308 deg; O4  -- O8  = 3 A
O4  -- T3  -- O9  = 108.618 deg; O4  -- O9  = 3 A
O4  -- T3  -- O10 = 114.934 deg; O4  -- O10 = 3 A
O8  -- T3  -- O9  = 108.677 deg; O8  -- O9  = 3 A
O8  -- T3  -- O10 = 108.923 deg; O8  -- O10 = 3 A
O9  -- T3  -- O10 = 106.196 deg; O9  -- O10 = 3 A
       106.196 deg <-- 109.442 deg --> 114.934 deg

O6  -- T4  -- O11 = 109.787 deg; O6  -- O11 = 3 A
O6  -- T4  -- O12 = 115.762 deg; O6  -- O12 = 3 A
O6  -- T4  -- O13 = 100.682 deg; O6  -- O13 = 3 A
O11 -- T4  -- O12 = 112.122 deg; O11 -- O12 = 3 A
O11 -- T4  -- O13 = 109.775 deg; O11 -- O13 = 3 A
O12 -- T4  -- O13 = 108.005 deg; O12 -- O13 = 3 A
       100.682 deg <-- 109.356 deg --> 115.762 deg

O7  -- T5  -- O14 = 113.683 deg; O7  -- O14 = 3 A
O7  -- T5  -- O15 = 106.727 deg; O7  -- O15 = 3 A
O7  -- T5  -- O16 = 105.807 deg; O7  -- O16 = 3 A
O14 -- T5  -- O15 = 110.137 deg; O14 -- O15 = 3 A
O14 -- T5  -- O16 = 110.410 deg; O14 -- O16 = 3 A
O15 -- T5  -- O16 = 109.915 deg; O15 -- O16 = 3 A
       105.807 deg <-- 109.446 deg --> 113.683 deg

O10 -- T6  -- O13 = 109.635 deg; O10 -- O13 = 3 A
O10 -- T6  -- O16 = 110.140 deg; O10 -- O16 = 3 A
O10 -- T6  -- O17 = 108.262 deg; O10 -- O17 = 3 A
O13 -- T6  -- O16 = 111.379 deg; O13 -- O16 = 3 A
O13 -- T6  -- O17 = 108.744 deg; O13 -- O17 = 3 A
O16 -- T6  -- O17 = 108.609 deg; O16 -- O17 = 3 A
       108.262 deg <-- 109.461 deg --> 111.379 deg

        O-T-O SUMMARY
          Range  = 86.6022 deg <--> 130.4441 deg
          Mean   = 109.3755 deg
          StdDev = 7.0173 deg

        O--O SUMMARY
          Range  = 2.1564 A <--> 2.9462 A
          Mean   = 2.6619 A
          StdDev = 0.1343 A

-------------------------------------------------------------------
------------------------- T-T-T Analysis --------------------------
-------------------------------------------------------------------
-------------------------------------------------------------------
------------------------- T-O-T Analysis --------------------------
-------------------------------------------------------------------
T1  -- O1  -- T1  = 169.077 deg ; T1  -- T1   3.2044 A

T1  -- O2  -- T1  = 111.742 deg ; T1  -- T1   2.7012 A

T1  -- O3  -- T2  = 109.569 deg ; T1  -- T2   2.5535 A

T1  -- O4  -- T3  = 172.963 deg ; T1  -- T3   3.2502 A

T2  -- O5  -- T2  = 159.772 deg ; T2  -- T2   3.1871 A

T2  -- O6  -- T4  = 121.852 deg ; T2  -- T4   2.9250 A

T2  -- O7  -- T5  = 144.602 deg ; T2  -- T5   3.1145 A

T3  -- O8  -- T3  = 133.079 deg ; T3  -- T3   2.9642 A

T3  -- O9  -- T3  = 149.617 deg ; T3  -- T3   3.0874 A

T3  -- O10 -- T6  = 164.374 deg ; T3  -- T6   3.2367 A

T4  -- O11 -- T4  = 163.886 deg ; T4  -- T4   3.3079 A

T4  -- O12 -- T4  = 159.255 deg ; T4  -- T4   3.3371 A

T4  -- O13 -- T6  = 124.000 deg ; T4  -- T6   2.9143 A

T5  -- O14 -- T5  = 152.355 deg ; T5  -- T5   3.2281 A

T5  -- O15 -- T5  = 131.338 deg ; T5  -- T5   2.9855 A

T5  -- O16 -- T6  = 145.483 deg ; T5  -- T6   3.1426 A

T6  -- O17 -- T6  = 147.086 deg ; T6  -- T6   3.1068 A


        T-O-T SUMMARY
          Range  = 109.5687° <--> 172.9632 deg
          Mean   = 144.7088 deg
          StdDev = 19.2143 deg

        T--T SUMMARY
          Range  = 2.5535 A <--> 3.3371 A
          Mean   = 3.0733 A
          StdDev = 0.2061 A

-------------------------------------------------------------------
------------------------ *** WARNINGS *** -------------------------
-------------------------------------------------------------------

SOME OXYGEN ATOMS ARE TOO CLOSE TO EACH OTHER
O3  -- O6  = 2.1564 A

T-T-T analysis was not conducted.

SOME T-ATOM DISTANCES ARE OUTSIDE THE NORMAL RANGE
T1  has 6 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T1  -- T1  = 3.2044 Angstrom
  T1  -- T1  = 2.7012 Angstrom
  T1  -- T2  = 2.5535 Angstrom
  T1  -- T4  = 3.4457 Angstrom
  T1  -- T2  = 3.3998 Angstrom
  T1  -- T3  = 3.2502 Angstrom
T2  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T2  -- T1  = 2.5535 Angstrom
  T2  -- T1  = 3.3998 Angstrom
  T2  -- T4  = 2.9250 Angstrom
  T2  -- T5  = 3.1145 Angstrom
  T2  -- T2  = 3.1871 Angstrom
T4  has 5 neighboring T-atoms within 3.50 A, but only 4 bridging O-atoms
  T4  -- T1  = 3.4457 Angstrom
  T4  -- T2  = 2.9250 Angstrom
  T4  -- T4  = 3.3079 Angstrom
  T4  -- T4  = 3.3371 Angstrom
  T4  -- T6  = 2.9143 Angstrom

-------------------------------------------------------------------
---------------------- Topological Analysis -----------------------
-------------------------------------------------------------------
T1 (Si): multiplicity = 24
Coordination Sequence =
    1 4 9 17 32 56 85 118 157 203 251 296 346 409 484 564 644
TD10 = 933
Circuit symbol = 4.4.4.6_{2}.6_{2}.6_{3}
Weight = 14
Vertex symbol  = 4.4.4.6_{2}.6.6_{2}
Weight = 14

T2 (Si): multiplicity = 24
Coordination Sequence =
    1 4 10 20 36 62 90 123 165 210 250 294 354 424 494 569 654
TD10 = 971
Circuit symbol = 4.4.6.6.6.6_{2}
Weight = 11
Vertex symbol  = 4.4.6.6.6.6_{2}
Weight = 11

T3 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 24 41 62 91 128 169 212 259 311 367 430 503 581 657
TD10 = 1002
Circuit symbol = 4.6.6.6_{4}.6.8_{5}
Weight = 24
Vertex symbol  = 4.6.6.6_{4}.6.8_{2}
Weight = 24

T4 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 24 42 65 94 128 165 206 256 313 371 432 502 580 658
TD10 = 996
Circuit symbol = 4.6.6.6_{2}.6.6_{2}
Weight = 18
Vertex symbol  = 4.6.6.6_{2}.6.6_{2}
Weight = 18

T5 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 25 44 66 93 125 161 203 255 314 373 434 504 582 661
TD10 = 988
Circuit symbol = 4.6.6.6_{2}.6_{2}.8_{5}
Weight = 24
Vertex symbol  = 4.6.6.6_{2}.6_{2}.8_{2}
Weight = 22

T6 (Si): multiplicity = 24
Coordination Sequence =
    1 4 11 24 43 68 95 122 157 206 259 310 374 450 511 565 648
TD10 = 990
Circuit symbol = 4.8_{4}.6_{3}.8_{4}.6_{3}.8_{4}
Weight = 30
Vertex symbol  = 4.8_{4}.6_{3}.8_{4}.6_{3}.8_{4}
Weight = 30

<TD10> = 980.000
Average ring size = 5.9512
